## On the Homogenization of 2D Porous Material with

## Determination of RVE

### Boutaani Mohamed said

1,2,a***, **

### Madani

### Salah

2,b### , Toufik kanit

2,c### and Fedaoui Kamel

2,d1 _{department of mechanics, University of Bejaia, 06000 Bejaia, Algeria }
2

Laboratory of Mechanical Structures and Materials, University of Batna 2, 05000 Batna, Algeria.

a _{mouhamed.boutaani@univ-begaia.dz }

**Abstract--****The numerical homogenization technique is used in **
**order to compute the effective elastic properties of heterogeneous **
**random 2-phase composites. Differents microstructures are **
**considered with different volume fraction. **

**microstructure with random distribution of identical **
**non-overlapping phases inclusions based on the Poisson process. **
**(PBC), boundary conditions are applied on the representative **
**volume element, RVE, of microstructures, for elastic modeling by **
**ﬁnite element method. The aim of the work was to examine how **
**spatial distribution and particles volume fraction influences the **
**elastic properties of the composite material. The results were **
**compared to various analytical model. **

**Index Term-- ****RVE, two-phase heterogeneous material, integral **
**range, numerical homogenization, statistical approach.**

INTRODUCTION

The homogenization of a heterogeneous material and analysis of its effective properties are classical problems in the micromechanics of heterogeneous material. There are many homogenization models, such as the inclusion model based on the Eshelby's solution, the direct averaging method and the two-scale expansion method Andrievski (2001) and Cailletaud (1994). The inclusion model can predict the effective properties depending on the volume fraction, geometrical size of the inclusion and constituent’s properties of composites. The the Hashin-Shtrikman model Hashin (1963) and the self-consistent scheme (SCM) Herve (1995) and Ostoja-Starzewski and Jeulin (2001) are developed along this line. They are widely applied to solve the eﬀective properties of various kinds of inhomogeneous materials.

A different way to solve homogenization problems is to use
numerical techniques and simulations on samples of the
microstructure. These techniques, used to estimate the
effective properties of random heterogeneous materials from
the constitutive law and the spatial distribution of different
components of the microstructure, are a main subject in the
mechanics of random materials. It is related to the
determination of the size of the representative volume element
(RVE) wich has been recentely studied widely with the
numerical and statistical tools (Sab, 2005a), (Tarada, 1998),
(Ostoja-Starzewski and Jeulin, 2001), and (Kanit et al., 2003).
The resulting apparent properties depend in fact on the choice
of boundary conditions used to impose mean strain, stress.
Three types of boundary conditions are classically used in
computational homogenization: kinematic uniform (*KUBC*),

stress uniform (*SUBC*) and Periodic boundary conditions
(*PERIODIC*).

The aim of our work is firstly the evaluation of effective
elastic properties of randomly distributed circular porous
inclusions and using the numerical homogenization cited in
(Kanit et al., 2006). Then we try to find a relationship between
the integral range and morphological properties of inclusions.
A quantitative definition of the RVE size based on the notion
of integral range is introduced. The *RVE* sizes found for the
different properties are compared. Their dependence on the
volume fraction and contrast properties is also discussed.

1 **GENERATE OF MICROSTRUCTURE AND MECHANICAL **
**PROPERTIES**

Different methods are commonly used for constructing random
microstructure volumes, the random sequential adsorption
(*RSA*) used in [22], [24] and [25], the Monte Carlo method in
[26], the molecular dynamics simulations in [20] and [27], and
the random-walk methods in the work of [28].

Fig. 1. Process of generating and meshing technic.

In this paper the randomly distributed forms of inclusions were generated in cell unit with an algorithm implemented in Python script, see figure 1. The volume fractions of forms inclusions used in this investigation are 10%, 30% and 50%. The condition of non-overlapping inclusions is imposed here with

Microstructure generating

Images generating

Code FE / FE Mesh

Superposition of finite element grid on the image

another condition that the inclusions do not hit any face of the
box. The computation numerical is used for generating images
used by the Code FE software*. *

**1.1 Material and description 1.2 Meshing **

We have chosen for our work, a model of microstructure
which constituted by two phases: one matrix (black color)
which is the hard phase and the second phase is constituted by
inclusions (in white color) (figure 2). These inclusions have a
form of circles, which distributed randomly. In this object, we
will use the following volume fractions: 0.10, 0.30 and 0.50 of
inclusions. We have generated several realizations of
microstructure for each volume fraction. These microstructures
will be use to determinate effective properties of the
heterogeneous material like the bulk and shear modulus*. *

Fig. 2. Equivalent Model of the homogeneous model for two-phase

The physical properties: Young's moduli (*E*), Poisson ratio (),
bulk (*K*) and shear (*µ*) modulus of matrix and inclusions, used
in the numerical simulations are given in table 1.

Table I

Physical properties of the material

Constitution *E*
[MPa]

[MPa]

*k*
[MPa]

*µ*
[MPa

]

Matrix 1000 0.3 9615 3846

Inclusion 10-8 0.49

**1.2 Meshing **

The finite element mesh associated with the image of the microstructure is obtained using the method of multi-phase elements see figure 2. A regular grid of 2D finite element is superimposed on an image of material. The mesh element is the quadratic with 4 nodes and integration complet.

Fig. 3. *Meshing microstructures*

2 EFFECTIVE LINEAR ELASTIC PROPERTIES

**2.1 Numerical homogenization**

The homogenization theory is used for the numerical determination of effective linear elasticity properties. A volume element of a heterogeneous material is considered.

Conditions are prescribed at its boundary in order to estimate
its overall properties. Two types of boundary conditions to be
prescribed on individual volume element are considered:
• Kinematic uniform boundary conditions (*KUBC*): the
displacement is imposed at point belonging to the boundary
such that :

*u*

### =

*E*

### .

*x*

###

*x*

###

###

*V*

(1)
*E* is a symmetrical second-rank tensor that does not depend on.
This implies that :

*E*

*dV*

*V*

*V*

### =

### 1

### >=

### <

###

###

###

(2)The symbol means equals by definition to. The macroscopic stress tensor is then defined by the spatial average:

*dV*

*V*

*V*

###

###

_{}

###

### =<

### >=

### 1

(3)• Periodicity conditions (PERIODIC): the displacement

field over the entire volume

*V*

takes the form :
###

###

*x*

*E*

*u*

### =

### .

(4)where the fluctuation

###

is periodic. It takes the same values at two homologous points on opposite faces of*V*. The traction

vector

*t*

### =

###

### .

*n*

takes opposite values at two homologous
points on opposite faces of *V*. By applying either macroscopic strain or stress, The local behaviour at every integration point inside each grain in the simulation is described by the fourth-rank linear elasticity tensor

*c*:

###

*x*

*c*

*x*

###

*x*

###

### =

### :

(5)We are used respectively to define the following ''apparent
bulk and shear modulus'' ( *k*app and µapp) :

> <

2 1 >= < 2 1 = >:

=< *E* *trace* 1122

*k* *k*

*app* (6)

> < 2 = >:

=< 12

*app* *E*_{} (7)
were <.> is the average value.

or for this case of *KUBC* and *PERIODIC* conditions
prescribed to a given volume *V*, one takes :

0 0 0

0 0 2 1

0 2 1 0

=

0 0 0

0 2 1 0

0 0 2 1

= *and* *E*_{}

*Ek*

(8)

**2.2 Variational bounds for the effective moduli of **
**heterogeneous **

To estimate the actual mechanical properties of a heterogeneous material, there are many methods of homogenization. We have used and tested the following methods : the bounds of Voigt and Reuss bounds of Hashin-Shtrikman optimal and the self-consistent model.

material, the Hashin-Shtrikman model (Hashin, 1963) is verified by:

###

###

1 1 11
1
2
1
3
4
1
= _{}
*k*
*P*
*k*
*k*
*P*
*k*

*kHS* (9)

###

###

###

###

1 1 1 1 1 1 2 1 3 4 5 2 2 1 = *k*

*k*

*P*

*P*

*HS* (10)

this conditions verified the property effectif for the materiel use.

The self-consistent estimate and the upper bound of (Zaoui, 1993) are used to determine the effective properties of the porous biphasic material :

###

###

###

###

###

###

###

1 2 1 2###

1
2
1
2
1
1
=
*k*
*k*
*P*
*k*
*k*
*k*
*P*
*k*
*k*
*keff*
(11)
*P*
*k*
*k*
*P*
*eff*
1
2
2
1
=
1
1
1
1
1
2
1
1

(12)

3 FLUCTUATION OF EFFECTIVE PROPERTIES AND DETERMINATION OF THE INTEGRAL RANGES

**3.1 Notion of Integral Range**

We consider fluctuations of average values over different
realizations of a random medium inside the domain *V*. In
geostatistics, it is well known that for an ergodic stationary

random function *Z*(x), one can compute the variance

*D*

*Z*2

### (

*V*

### )

of its average value *Z*(x) over the volume *V* as a function of
the central covariance function *Q*(h) of *Z*(x) by :

_{Q}_{x}_{y}_{dxdy}

*V*
*V*
*D*

*V*
*V*

*Z* ( )

1 = )

( _{2}

2

###

###

(13)For a large specimen (with V>>A2), Eq. (13) can be expressed

to the first order in *1/V* as a function of the integral range in
the space *R*2, *A*2, by (Matheron, 1971) and (Lantuejoul, 1991) :

*V*
*A*
*D*
*V*

*D _{Z}*2

*2 2*

_{Z}= )

( (14)

with
*dh*
*h*
*Q*
*D*
*A*
*R*
*Z*
)
(
1

= _{2} _{2}

2

###

Where 2

*Z*

*D* is the point variance of *Z*(x) and *A*2 is the integral

range of the random function *Z*(x).

The scaling Eq. (14) is valid for an additive combination of the
variable *Z* over the region of interest *V*, when its size is such
that *V* > *A*2 and when *A*2 is finite. For an infinite integral

range, *V* can be replaced in many cases by *V* (with * ≠ 1*) in
Eq. (14) (Lantuejoul, 1991).

As the composition of elastic moduli in the change of scale is not additive in general, relation (14) cannot be applied. Instead we propose, as (Cailletaud et al., 2003), to test a power law according to the relation :

) ( = )

( 2 2

2

*V*
*A*
*D*
*V*

*DZ* *Z* (15)

A similar relation was proposed and tested by (Cailletaud et
al., 1994) and (Kanit et al., 2003). In the case of a two-phase
material with elastic property *Z*1 for phase 1 and *Z*2 for phase

2, the point variance

*D*

*Z*2 of the random variable Z is given by :

*D*

*Z*2

### =

*P*

### (1

###

*P*

### )(

*Z*

_{1}

###

*Z*

_{2}

### )

2 (16) with: • *P* and (*1-P*) are the volume fraction of inclusions and
matrix respectively

• *Z*1 and *Z*2 are the properties elastic (*k* or µ)of inclusions

and matrix respectively The Eq. (16) becomes :

*V*
*A*
*Z*
*Z*
*P*
*P*
*V*
*DZ*
2
2
2
1
2
.
)
)(
(1
=
)

( (17)

**3.2 Dispersions of physical Properties **

The numerical simulations based on the finite element method
are carried out for two different boundary conditions:
kinematic uniform boundary conditions (*KUBC*) and the
periodic boundary conditions (*PERIODIC*). The studied
volume fraction of inclusion phase is (*P =0.10, P =0.30, P *
*=0.50*) and the number of realizations for each volume is one
realization. which is the wanted effective modulus.

It can be noticed that the mean value given by the periodic boundary conditions varies slightly as a function of the size of the domain, as compared to the other boundary conditions. Figures 4, 5 and 6 gives the corresponding confidence

intervals

### [

*Z*

###

### 2

*D*

*Z*

### ,

*Z*

###

### 2

*D*

*Z*

### ]

, where Z is one of theapparent moduli,

_{Z}

its mean value and _{Z}

*DZ*2(

*V*) its variance.

This three curves for the case of periodic boundary condition
and *SCM* model.

The obtained mean values generally depend on the volume
size, but also on the type of boundary conditions. For each
modulus, the values converge towards the same limit for large
volumes *V* (*V* is the numbre of inclusions), which is the wanted
effective modulus. The values *k*eff, *µ*eff and *E*eff found for large
volume sizes are reported in table. II and compared to the
Voigt-Reuss (upper bound and lower bound),
Hashin-Shtrikman's bounds (*HS*+ and *HS*-) and (*SCM*) (Christensen,
1979a), also given in table II :

Table II

Values of numerical resultants, VR Bounds, HS Bounds and SCM for effective elastic properties of two phase heterogeneous porous material

*Properties * *Simul.* *Voigt* *HS+* *SCM*

*k*(P = 0.10) 2822 8653 7287 6923

*µ*(P = 0.10) 2917 3461 3221 2933

*k*(P = 0.30) 3725 6730 4307 3846

*µ*(P = 0.30) 1633 2692 2223 1748

*k*(P = 0.50) 1922 4807 2481 2136

Table III

Integral range for k and µ modulus

*A*(*k*) *A*(*µ*)

*P* = 0.10 0.0039 0.0045

*P* = 0.30 0.0017 0.0021

*P* = 0.50 0.00027 0.00018

Fig. 4. *A figure title; *Convergence curve of the RVE and dispersion and mean
value of the apparent elastic properties as a function of the domain size for
periodic boundary conditions in the case (*P*=0.10) : a) evolution of *k*app ; and

b) evolution of µapp.

Fig. 5. *A figure title; *Convergence curve of the RVE and dispersion and mean
value of the apparent elastic properties as a function of the domain size for
periodic boundary conditions in the case (*P*=0.30) : a) evolution of *k*app _{; and }

b) evolution of µapp_{. }

Fig. 6. *A figure title; *Convergence curve of the RVE and dispersion and mean
value of the apparent elastic properties as a function of the domain size for
periodic boundary conditions in the case (*P*=0.50) : a) evolution of *k*app ; and

**3.3 Representative Volume Elementary Size **

In this part we represent the table are obtained by
simulation of elastic properites volume function *V*. The results
is obtained by fitting the mathematical model with the
simulation curves of *k*app and *µ*app, or :

*V*
*A*
*D*
*k*

*rel*
*Z*
*eff*

3 2

= (18)

Or *DZ* is the variance of *k* modulus : *DZ* = *Dk* and ;

*V*
*A*
*D*

*rel*
*Z*
*eff*

2 3

= (19)

or *DZ* is the variance of *µ* modulus : *DZ* = *Dµ.* The numerical

results of simulation of physical properties corresponds to the
model mathematical (18) and (19) gives the following table.
The size of the RVE can now be defined as the volume for
which for instance n = 1 realization is necessary to estimate the
mean property *Z* with a relative error a = 1%, provided we
now the function *DZ* (*V*) :

This table shows the property A2 for the three volume fractions

in both cases (*k* and *µ*). The integral range A2 depend only on

the volume fraction of the inclusion. We have seen in all the
cases studies here that the others parametrers have no relation
and influence on the integral range. Integral range *A*2 can be

found by using the proposed relation :

*A*

_{2}

### =

*P*

### /

*RVE*

(20)
for the exemple studies in this paper, we have :
• *P=0.10*, *RVE =20* inclusions

• *P=0.30*, *RVE =100* inclusions
• *P=0.50*, *RVE =200* inclusions

Figure 6 sumarize the evolution of the RVE with the volume fraction of the inclusion.

Fig. 7. Evolution of the RVE with the volume fraction

**3.4 EFFECT OF THE VOLUME FRACTION AND CONTRAST ON **
**THE INTEGRAL RANGES**

The apparent properties and integral ranges obtained for
elasticity depend on the volume fraction of phases and the
representative elementary volume (*RVE*). In this section, we

come back to the variance

*D*

*z*2 of the effective properties for

the phases elastic material, which is Eq. (17), in the two-dimensional it becomes :

###

###

###

*RVE*

*A*

*k*

*k*

*P*

*P*

*D*

*2 2*

_{z}2 1 2

### 1

### =

###

###

It was found that the quantity: *A2 = P/RVE*, implies :

###

###

###

2 2 2 1 2

### 1

### =

*RVE*

*P*

*k*

*k*

*P*

*P*

*D*

*k*

###

###

(21)and

###

###

###

2_{2}

2 1 2

1 =

*RVE*
*P*
*P*

*P*

*D*_{}

###

###

(22)so, for the contrast c = *k*2/*k*1 => *k*2 = c.*k*1

(*k*1: matrix and *k*2 : inclusion)

for example :
If* k*1 = 1, (18) implies:

###

###

###

22 2

1

2_{=} _{.} _{1} _{1}

*RVE*
*P*
*c*
*P*
*k*
*P*

*D _{k}* (23)

for the model is converge it is necessary that the variance

*D*

*k*2

takes the minimum (ie :

*D*

*k*2

### =

### 1

) implies###

###

###

2_{2}

2 1

2

### 1

### 1

### 1

### .

### =

### 1

*RVE*

*c*

*P*

*k*

*P*

###

###

or:

*RVE*

### =

*P*

### .

### |

### 1

###

*c*

### |

### .

### 1

###

*P*

(24)
it is the relationship between RVE and contrast (*RVE = f(c)*)

The relation :

*RVE*

### =

*P*

### |

### 1

###

*c*

### |

### 1

###

*P*

equivalent of relation :
###

*c*

*P*

*c*

*P*

*f*

*y*

### =

### =

### |

### 1

###

### |

### 1

###

Or, to plot the three cases we study the contrast : *c < 1* matrix stiffer than the inclusion

*c = 1* matrix stiffer than the inclusion

*c > 1* inclusion stiffer than the matrix

so for *P=0.3* the curve *y =f(c) *is represented as follows:

- when c=0 the *RVE* is equal to the value

*P*

### .

### 1

###

*P*

### .

*k*

1 or the
RVE depends on the volume fraction and the property *k*1 of the

matrix.

when *c=1* the *RVE=0* that mean that the properties of the two
phases are equal implies *k*2 =* k*1,

- when *RVE ** I* implies *k*2 <* k*1, when th contrast *0 < c <1 * and
*RVERPM < RVE < 1* (*RVERPM* is the *RVE* for porous media),

media matrix is more compressible than for the inclusion.
- when *RVE ** II* implies* k*1 <* k*2, when the contrast *c > 1*, the

media for inclusions is more compressible than for the matrix.

CONCLUSIONS

The effective linear properties of random materials can be determined not only by numerical simulations on large volume elements of heterogeneous material, but also as mean values of apparent properties of rather small volumes, providing that a sufficient number of realizations is considered. This is very important, since computations on large volumes are usually prohibitive. This corresponds also to an enlarged definition of representative volume element. Its size mustbe considered as a function of five parameters: the physical property, the contrast of properties, the volume fractions of components, the wanted relative precision for the estimation of the effective property and the number of realizations of the microstructure associated with computations that one is ready to carry out. It depends also in fine on the special morphology of distribution of The integral range is of importance in the study of homogenization of microstructures and for the determination of effective properties of materials, this property is a quantity morphological and for the case of porous material, it depend only on volume fraction of inclusion. the proposed relation (20) for the determiantion of the value of integral range complate the methodology proposed by (Kanit et al., 2003). The contrast between the two phases is very importante on the behaviour of the porous material, this question is investigated and developped in the last section and need to be study more. we soulved three great point from the study of the contrast :

• contrast *c = 0*⇒ porous material
• contrast *c *∈* ]0, 1[*⇒ porous material

• contrast *c =1* ⇒ RVE d’ont exist or material
incompressible

• contrast *c >1*⇒ the behaviour of the material depend
on the inclusion.

REFERENCES

[1] Kanit, T., Forest, S., Galliet, I., Mounoury, V., Jeulin, D. (2003). Determination of the size of the representative volume element for random composites: statistical and numerical approach. Methods in applied mechanics and engineering, Vol. 195, p. 3960–3982, [2] Kanit, T., N’Guyen, F., Forest, S. Jeulin, D., Reed, M., Singleton,

S. (2006). Apparent and eﬀective physical properties of heterogeneous materials: Representativity of samples of two materials from food industry. Int. Journal of Solids and Structures. Vol. 40, p. 3647–3679.

[3] Jeulin, D., (2001). Caractérisation Morphologique et modèles de Structures Aléatoires, Homogénéisation en mécanique des matériaux (tome1). Hermès, France.

[4] Ghossein E. and Lévesque M. (2014). A comprehensive validation of analytical homogenization models: The case of ellipsoidal particles reinforced composites, Mechanics of Materials, 75, p. 135-150.

[5] Moussaddy, H., Therriault, D., Lévesque, M. (2013). Submitted to: “International Journal of Solids and Structures. Assessment of existing and introduction of a new and robust efficient definition of the representative volume element.

[6] Pahlavan, M., Moussaddy, H., Ghossein, E. (2013). Prediction of Elastic Properties in Polymer-Clay Nanocomposites: Analytical Homogenization Methods and 3D Finite Element Modeling. Computational Materials Science.

[7] Cailletaud, G. (1994). Size eﬀects on elastic properties of random composites. Engineering Computations. Vol. 11, p. 99–110. [8] G. Cailletaud, S., Forest, D., Jeulin, F., Feyel, I., Galliet, V.,

Mounoury, S. (2003). Quilici, Some elements of microstructural mechanics. Comput. Mater. Sci Vol. 27, p. 351–374.

[9] Christensen, R. (1979a). Solutions for eﬀective shear properties of three phase sphere and cylinder models. Journal of the Mechanics and Physics of solids, Vol. 271, p. 315–330.

[10] Hashin, Z.S. (1963). A variational approach to the theory of elastic behaver of multiphase materials. J. Mech Phys Solids Vol. 11, p. 127–140.

[11] Herve, E., Zaoui, A. (1995). Elastic behaver of multiply coated ﬁber-reinforced composites. Inter. Journal of Engineering Sciences Vol. 33, p. 1419–1433.

[12] Lantuejoul, C. (1991). Ergodicity and integral range. Journal of Microscopy 161, p. 387–403.

[13] Matheron, G. (1971). The theory of regionalized variables and its applications. Paris school of mines publications.